General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 8.79 - 8.8 g/cm³ Show Material materials with Density of 8.79 - 8.8 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | 20.0 °C | 124 GPa Show Material materials with Elastic modulus of 124 GPa |

100.0 °C | 123 GPa Show Material materials with Elastic modulus of 123 GPa | |

200.0 °C | 118 GPa Show Material materials with Elastic modulus of 118 GPa | |

300.0 °C | 113 GPa Show Material materials with Elastic modulus of 113 GPa | |

400.0 °C | 107 GPa Show Material materials with Elastic modulus of 107 GPa | |

500.0 °C | 98 GPa Show Material materials with Elastic modulus of 98 GPa | |

600.0 °C | 88 GPa Show Material materials with Elastic modulus of 88 GPa | |

700.0 °C | 78 GPa Show Material materials with Elastic modulus of 78 GPa | |

Hardness, Brinell | 20.0 °C | 90 - 120 [-] Show Material materials with Hardness, Brinell of 90 - 120 [-] |

Poisson's ratio | 20.0 °C | 0.34 [-] Show Material materials with Poisson's ratio of 0.34 [-] |

Shear modulus | 20.0 °C | 46 GPa Show Material materials with Shear modulus of 46 GPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | 200.0 °C | 1.9E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.9E-5 1/K | |

Melting point | 875 - 1075 °C Show Material materials with Melting point of 875 - 1075 °C | Typical for Wrought Copper Brass | |

Specific heat capacity | 20.0 °C | 376 - 377 J/(kg·K) Show Material materials with Specific heat capacity of 376 - 377 J/(kg·K) | |

100.0 °C | 398 J/(kg·K) Show Material materials with Specific heat capacity of 398 J/(kg·K) | ||

200.0 °C | 410 J/(kg·K) Show Material materials with Specific heat capacity of 410 J/(kg·K) | ||

300.0 °C | 419 J/(kg·K) Show Material materials with Specific heat capacity of 419 J/(kg·K) | ||

400.0 °C | 431 J/(kg·K) Show Material materials with Specific heat capacity of 431 J/(kg·K) | ||

500.0 °C | 444 J/(kg·K) Show Material materials with Specific heat capacity of 444 J/(kg·K) | ||

600.0 °C | 452 J/(kg·K) Show Material materials with Specific heat capacity of 452 J/(kg·K) | ||

700.0 °C | 465 J/(kg·K) Show Material materials with Specific heat capacity of 465 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 184 W/(m·K) Show Material materials with Thermal conductivity of 184 W/(m·K) | |

80.0 °C | 197 W/(m·K) Show Material materials with Thermal conductivity of 197 W/(m·K) | ||

120.0 °C | 209 W/(m·K) Show Material materials with Thermal conductivity of 209 W/(m·K) | ||

160.0 °C | 218 W/(m·K) Show Material materials with Thermal conductivity of 218 W/(m·K) | ||

200.0 °C | 226 W/(m·K) Show Material materials with Thermal conductivity of 226 W/(m·K) | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical conductivity | 20.0 °C | 2.47E+7 - 2.50E+7 S/m Show Material materials with Electrical conductivity of 2.47E+7 - 2.50E+7 S/m |

Electrical resistivity | 20.0 °C | 4.1E-8 Ω·m Show Material materials with Electrical resistivity of 4.1E-8 Ω·m |

Specific Electrical conductivity | 43 % IACS Show Material materials with Specific Electrical conductivity of 43 % IACS |

Chemical properties

Property | Value |
---|---|

Aluminium | 0.02 % Show Material materials with Aluminium of 0.02 % |

Copper | 89 - 91 % Show Material materials with Copper of 89 - 91 % |

Iron | 0.05 % Show Material materials with Iron of 0.05 % |

Lead | 0.05 % Show Material materials with Lead of 0.05 % |

Nickel | 0.3 % Show Material materials with Nickel of 0.3 % |

Tin | 0.1 % Show Material materials with Tin of 0.1 % |